#------------------------------------------------------------------------------
#$Date: 2016-02-18 17:37:37 +0200 (Thu, 18 Feb 2016) $
#$Revision: 176729 $
#$URL: svn://www.crystallography.net/cod/cif/1/50/84/1508443.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1508443
loop_
_publ_author_name
'He, Hua'
Tyson,Chauntae
'Bobev, Svilen'
_publ_section_title
;
 Synthesis and Crystal Structures of the Quaternary Zintl Phases
 RbNa8Ga3Pn6 (Pn = P, As) and Na10NbGaAs6
;
_journal_issue                   2
_journal_name_full               Crystals
_journal_page_first              213
_journal_page_last               223
_journal_paper_doi               10.3390/cryst2020213
_journal_volume                  2
_journal_year                    2012
_chemical_formula_moiety         'As6 Ga3, Rb, 8(Na)'
_chemical_formula_sum            'As6 Ga3 Na8 Rb'
_chemical_formula_weight         928.07
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   22.843(6)
_cell_length_b                   4.7892(12)
_cell_length_c                   16.861(4)
_cell_measurement_reflns_used    2575
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      28.33
_cell_measurement_theta_min      1.50
_cell_volume                     1844.6(8)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      200(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0888
_diffrn_reflns_av_sigmaI/netI    0.0428
_diffrn_reflns_limit_h_max       30
_diffrn_reflns_limit_h_min       -30
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            24813
_diffrn_reflns_theta_full        28.33
_diffrn_reflns_theta_max         28.33
_diffrn_reflns_theta_min         1.50
_exptl_absorpt_coefficient_mu    17.814
_exptl_absorpt_correction_T_max  0.641
_exptl_absorpt_correction_T_min  0.532
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS (Sheldrick, 2003)
;
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    3.342
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       bar
_exptl_crystal_F_000             1664
_exptl_crystal_size_max          0.070
_exptl_crystal_size_mid          0.030
_exptl_crystal_size_min          0.025
_refine_diff_density_max         1.164
_refine_diff_density_min         -0.928
_refine_diff_density_rms         0.215
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.031
_refine_ls_matrix_type           full
_refine_ls_number_parameters     109
_refine_ls_number_reflns         2575
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.031
_refine_ls_R_factor_all          0.0619
_refine_ls_R_factor_gt           0.0326
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0163P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0521
_refine_ls_wR_factor_ref         0.0611
_reflns_number_gt                1806
_reflns_number_total             2575
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            RbNa8Ga3As6_crystals-02-00213-s001_DC181.cif
_cod_data_source_block           I_chateigner_1508443
_cod_depositor_comments          'mistake in journal_issue, fixed'
_cod_database_code               1508443
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z'
'-x-1/2, y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Rb Rb 0.00193(3) 0.2500 0.69125(4) 0.01864(15) Uani 1 2 d S
Na1 Na 0.05179(12) 0.2500 0.46701(16) 0.0199(7) Uani 1 2 d S
Na2 Na 0.05669(12) 0.2500 0.14932(17) 0.0199(7) Uani 1 2 d S
Na3 Na 0.17952(14) 0.2500 0.57880(17) 0.0235(7) Uani 1 2 d S
Na4 Na 0.18164(12) 0.2500 0.80793(18) 0.0223(6) Uani 1 2 d S
Na5 Na 0.19078(13) 0.2500 0.04272(17) 0.0229(7) Uani 1 2 d S
Na6 Na 0.33734(12) 0.2500 0.70089(17) 0.0208(7) Uani 1 2 d S
Na7 Na 0.34121(13) 0.2500 0.91856(17) 0.0224(7) Uani 1 2 d S
Na8 Na 0.54046(12) 0.2500 0.55567(18) 0.0225(7) Uani 1 2 d S
Ga1 Ga 0.21495(3) 0.2500 0.30917(5) 0.01302(16) Uani 1 2 d S
Ga2 Ga 0.36418(3) 0.2500 0.43088(5) 0.01279(17) Uani 1 2 d S
Ga3 Ga 0.37259(3) 0.2500 0.19041(5) 0.01285(16) Uani 1 2 d S
As1 As 0.11275(3) 0.2500 0.30823(4) 0.01406(15) Uani 1 2 d S
As2 As 0.25997(3) 0.2500 0.43702(5) 0.01991(18) Uani 1 2 d S
As3 As 0.26682(3) 0.2500 0.18538(5) 0.01781(17) Uani 1 2 d S
As4 As 0.41057(3) 0.2500 0.55534(4) 0.01423(16) Uani 1 2 d S
As5 As 0.41739(3) 0.2500 0.06487(4) 0.01355(16) Uani 1 2 d S
As6 As 0.42487(3) 0.2500 0.31535(5) 0.01653(16) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
As1 Rb As1 84.86(3) 5_556 5_566
As1 Rb As6 142.35(3) 5_556 2_565
As1 Rb As6 83.82(2) 5_566 2_565
As1 Rb As6 83.82(2) 5_556 2
As1 Rb As6 142.35(3) 5_566 2
As6 Rb As6 83.59(3) 2_565 2
As1 Rb As5 86.12(2) 5_556 2
As1 Rb As5 143.73(3) 5_566 2
As6 Rb As5 122.36(3) 2_565 2
As6 Rb As5 70.85(2) 2 2
As1 Rb As5 143.73(3) 5_556 2_565
As1 Rb As5 86.12(2) 5_566 2_565
As6 Rb As5 70.85(2) 2_565 2_565
As6 Rb As5 122.36(3) 2 2_565
As5 Rb As5 80.73(3) 2 2_565
As1 Rb Ga3 177.442(16) 5_556 2_565
As1 Rb Ga3 97.70(2) 5_566 2_565
As6 Rb Ga3 38.532(19) 2_565 2_565
As6 Rb Ga3 94.15(3) 2 2_565
As5 Rb Ga3 91.75(3) 2 2_565
As5 Rb Ga3 36.879(19) 2_565 2_565
As1 Rb Ga3 97.70(2) 5_556 2
As1 Rb Ga3 177.442(16) 5_566 2
As6 Rb Ga3 94.15(3) 2_565 2
As6 Rb Ga3 38.532(19) 2 2
As5 Rb Ga3 36.879(19) 2 2
As5 Rb Ga3 91.75(3) 2_565 2
Ga3 Rb Ga3 79.75(3) 2_565 2
As1 Rb Na1 48.42(4) 5_556 5_556
As1 Rb Na1 100.90(4) 5_566 5_556
As6 Rb Na1 169.10(5) 2_565 5_556
As6 Rb Na1 98.03(3) 2 5_556
As5 Rb Na1 49.18(4) 2 5_556
As5 Rb Na1 99.49(4) 2_565 5_556
Ga3 Rb Na1 130.62(5) 2_565 5_556
Ga3 Rb Na1 80.84(4) 2 5_556
As1 Rb Na1 100.90(4) 5_556 5_566
As1 Rb Na1 48.42(4) 5_566 5_566
As6 Rb Na1 98.03(3) 2_565 5_566
As6 Rb Na1 169.10(5) 2 5_566
As5 Rb Na1 99.49(4) 2 5_566
As5 Rb Na1 49.18(4) 2_565 5_566
Ga3 Rb Na1 80.84(4) 2_565 5_566
Ga3 Rb Na1 130.62(5) 2 5_566
Na1 Rb Na1 78.38(6) 5_556 5_566
As1 Rb Na2 99.30(4) 5_556 5_566
As1 Rb Na2 47.19(4) 5_566 5_566
As6 Rb Na2 48.63(4) 2_565 5_566
As6 Rb Na2 99.79(4) 2 5_566
As5 Rb Na2 168.77(5) 2 5_566
As5 Rb Na2 99.98(3) 2_565 5_566
Ga3 Rb Na2 82.56(4) 2_565 5_566
Ga3 Rb Na2 132.05(5) 2 5_566
Na1 Rb Na2 140.71(6) 5_556 5_566
Na1 Rb Na2 89.20(5) 5_566 5_566
As1 Rb Na2 47.19(4) 5_556 5_556
As1 Rb Na2 99.30(4) 5_566 5_556
As6 Rb Na2 99.79(4) 2_565 5_556
As6 Rb Na2 48.63(4) 2 5_556
As5 Rb Na2 99.98(3) 2 5_556
As5 Rb Na2 168.77(5) 2_565 5_556
Ga3 Rb Na2 132.05(5) 2_565 5_556
Ga3 Rb Na2 82.56(4) 2 5_556
Na1 Rb Na2 89.20(5) 5_556 5_556
Na1 Rb Na2 140.71(6) 5_566 5_556
Na2 Rb Na2 77.13(6) 5_566 5_556
As5 Na1 As5 106.32(9) 2_565 2
As5 Na1 As1 112.38(6) 2_565 .
As5 Na1 As1 112.38(6) 2 .
As5 Na1 As5 109.08(6) 2_565 6_556
As5 Na1 As5 109.08(6) 2 6_556
As1 Na1 As5 107.55(9) . 6_556
As5 Na1 Na3 60.21(5) 2_565 .
As5 Na1 Na3 60.21(5) 2 .
As1 Na1 Na3 95.38(9) . .
As5 Na1 Na3 157.07(11) 6_556 .
As5 Na1 Na7 54.54(5) 2_565 2_564
As5 Na1 Na7 120.62(10) 2 2_564
As1 Na1 Na7 58.22(6) . 2_564
As5 Na1 Na7 130.11(7) 6_556 2_564
Na3 Na1 Na7 62.77(7) . 2_564
As5 Na1 Na7 120.62(10) 2_565 2_554
As5 Na1 Na7 54.54(5) 2 2_554
As1 Na1 Na7 58.22(6) . 2_554
As5 Na1 Na7 130.11(7) 6_556 2_554
Na3 Na1 Na7 62.77(7) . 2_554
Na7 Na1 Na7 85.80(9) 2_564 2_554
As5 Na1 Na1 121.63(12) 2_565 5_556
As5 Na1 Na1 56.18(5) 2 5_556
As1 Na1 Na1 125.90(9) . 5_556
As5 Na1 Na1 52.90(7) 6_556 5_556
Na3 Na1 Na1 112.97(11) . 5_556
Na7 Na1 Na1 175.06(14) 2_564 5_556
Na7 Na1 Na1 94.41(5) 2_554 5_556
As5 Na1 Na1 56.18(5) 2_565 5_566
As5 Na1 Na1 121.63(12) 2 5_566
As1 Na1 Na1 125.90(9) . 5_566
As5 Na1 Na1 52.90(7) 6_556 5_566
Na3 Na1 Na1 112.97(11) . 5_566
Na7 Na1 Na1 94.41(5) 2_564 5_566
Na7 Na1 Na1 175.06(14) 2_554 5_566
Na1 Na1 Na1 84.97(12) 5_556 5_566
As5 Na1 Rb 165.99(7) 2_565 5_556
As5 Na1 Rb 87.64(3) 2 5_556
As1 Na1 Rb 61.62(5) . 5_556
As5 Na1 Rb 63.87(5) 6_556 5_556
Na3 Na1 Rb 130.85(6) . 5_556
Na7 Na1 Rb 119.45(9) 2_564 5_556
Na7 Na1 Rb 68.36(6) 2_554 5_556
Na1 Na1 Rb 65.05(6) 5_556 5_556
Na1 Na1 Rb 115.57(12) 5_566 5_556
As5 Na1 Rb 87.64(3) 2_565 5_566
As5 Na1 Rb 165.99(7) 2 5_566
As1 Na1 Rb 61.62(5) . 5_566
As5 Na1 Rb 63.87(5) 6_556 5_566
Na3 Na1 Rb 130.85(6) . 5_566
Na7 Na1 Rb 68.36(6) 2_564 5_566
Na7 Na1 Rb 119.45(9) 2_554 5_566
Na1 Na1 Rb 115.57(12) 5_556 5_566
Na1 Na1 Rb 65.05(6) 5_566 5_566
Rb Na1 Rb 78.38(6) 5_556 5_566
As5 Na1 Rb 62.60(5) 2_565 .
As5 Na1 Rb 62.60(5) 2 .
As1 Na1 Rb 169.28(10) . .
As5 Na1 Rb 83.17(6) 6_556 .
Na3 Na1 Rb 73.90(7) . .
Na7 Na1 Rb 115.01(7) 2_564 .
Na7 Na1 Rb 115.01(7) 2_554 .
Na1 Na1 Rb 60.46(8) 5_556 .
Na1 Na1 Rb 60.46(8) 5_566 .
Rb Na1 Rb 125.51(6) 5_556 .
Rb Na1 Rb 125.51(6) 5_566 .
As4 Na2 As4 107.61(9) 2_554 2_564
As4 Na2 As1 111.91(7) 2_554 .
As4 Na2 As1 111.91(7) 2_564 .
As4 Na2 As6 110.54(7) 2_554 6_556
As4 Na2 As6 110.54(7) 2_564 6_556
As1 Na2 As6 104.36(9) . 6_556
As4 Na2 Na8 59.73(5) 2_554 6_556
As4 Na2 Na8 59.73(5) 2_564 6_556
As1 Na2 Na8 160.58(11) . 6_556
As6 Na2 Na8 95.07(9) 6_556 6_556
As4 Na2 Na6 120.56(10) 2_554 2_564
As4 Na2 Na6 53.74(5) 2_564 2_564
As1 Na2 Na6 58.65(6) . 2_564
As6 Na2 Na6 128.88(7) 6_556 2_564
Na8 Na2 Na6 108.63(8) 6_556 2_564
As4 Na2 Na6 53.74(5) 2_554 2_554
As4 Na2 Na6 120.56(10) 2_564 2_554
As1 Na2 Na6 58.65(6) . 2_554
As6 Na2 Na6 128.88(7) 6_556 2_554
Na8 Na2 Na6 108.63(8) 6_556 2_554
Na6 Na2 Na6 85.91(9) 2_564 2_554
As4 Na2 Na5 60.81(5) 2_554 .
As4 Na2 Na5 60.81(5) 2_564 .
As1 Na2 Na5 94.86(9) . .
As6 Na2 Na5 160.79(11) 6_556 .
Na8 Na2 Na5 65.72(8) 6_556 .
Na6 Na2 Na5 62.04(7) 2_564 .
Na6 Na2 Na5 62.04(7) 2_554 .
As4 Na2 Na8 52.33(5) 2_554 2_554
As4 Na2 Na8 117.04(10) 2_564 2_554
As1 Na2 Na8 131.05(6) . 2_554
As6 Na2 Na8 58.95(6) 6_556 2_554
Na8 Na2 Na8 60.12(7) 6_556 2_554
Na6 Na2 Na8 168.28(11) 2_564 2_554
Na6 Na2 Na8 94.55(5) 2_554 2_554
Na5 Na2 Na8 107.90(8) . 2_554
As4 Na2 Na8 117.04(10) 2_554 2_564
As4 Na2 Na8 52.33(5) 2_564 2_564
As1 Na2 Na8 131.05(6) . 2_564
As6 Na2 Na8 58.95(6) 6_556 2_564
Na8 Na2 Na8 60.12(7) 6_556 2_564
Na6 Na2 Na8 94.55(5) 2_564 2_564
Na6 Na2 Na8 168.28(11) 2_554 2_564
Na5 Na2 Na8 107.90(8) . 2_564
Na8 Na2 Na8 82.65(9) 2_554 2_564
As4 Na2 Rb 164.74(7) 2_554 5_566
As4 Na2 Rb 87.62(3) 2_564 5_566
As1 Na2 Rb 61.24(5) . 5_566
As6 Na2 Rb 61.46(5) 6_556 5_566
Na8 Na2 Rb 131.20(6) 6_556 5_566
Na6 Na2 Rb 69.03(6) 2_564 5_566
Na6 Na2 Rb 119.45(9) 2_554 5_566
Na5 Na2 Rb 130.91(6) . 5_566
Na8 Na2 Rb 120.21(9) 2_554 5_566
Na8 Na2 Rb 71.32(5) 2_564 5_566
As4 Na2 Rb 87.62(3) 2_554 5_556
As4 Na2 Rb 164.74(7) 2_564 5_556
As1 Na2 Rb 61.24(5) . 5_556
As6 Na2 Rb 61.46(5) 6_556 5_556
Na8 Na2 Rb 131.20(6) 6_556 5_556
Na6 Na2 Rb 119.45(9) 2_564 5_556
Na6 Na2 Rb 69.03(6) 2_554 5_556
Na5 Na2 Rb 130.91(6) . 5_556
Na8 Na2 Rb 71.32(5) 2_554 5_556
Na8 Na2 Rb 120.21(9) 2_564 5_556
Rb Na2 Rb 77.13(6) 5_566 5_556
As2 Na3 As3 102.10(7) . 2_565
As2 Na3 As3 102.10(7) . 2
As3 Na3 As3 95.50(8) 2_565 2
As2 Na3 As5 110.84(7) . 2
As3 Na3 As5 146.98(10) 2_565 2
As3 Na3 As5 75.78(3) 2 2
As2 Na3 As5 110.84(7) . 2_565
As3 Na3 As5 75.78(3) 2_565 2_565
As3 Na3 As5 146.98(10) 2 2_565
As5 Na3 As5 94.17(9) 2 2_565
As2 Na3 Ga3 132.70(4) . 2_565
As3 Na3 Ga3 43.63(3) 2_565 2_565
As3 Na3 Ga3 111.12(9) 2 2_565
As5 Na3 Ga3 109.34(9) 2 2_565
As5 Na3 Ga3 42.14(3) 2_565 2_565
As2 Na3 Ga3 132.70(4) . 2
As3 Na3 Ga3 111.12(9) 2_565 2
As3 Na3 Ga3 43.63(3) 2 2
As5 Na3 Ga3 42.14(3) 2 2
As5 Na3 Ga3 109.34(9) 2_565 2
Ga3 Na3 Ga3 94.16(8) 2_565 2
As2 Na3 Na1 94.68(9) . .
As3 Na3 Na1 128.29(6) 2_565 .
As3 Na3 Na1 128.29(6) 2 .
As5 Na3 Na1 52.58(5) 2 .
As5 Na3 Na1 52.58(5) 2_565 .
Ga3 Na3 Na1 90.37(7) 2_565 .
Ga3 Na3 Na1 90.37(7) 2 .
As2 Na3 Na7 59.40(6) . 2_554
As3 Na3 Na7 161.49(11) 2_565 2_554
As3 Na3 Na7 88.55(4) 2 2_554
As5 Na3 Na7 51.46(5) 2 2_554
As5 Na3 Na7 109.89(9) 2_565 2_554
Ga3 Na3 Na7 149.46(11) 2_565 2_554
Ga3 Na3 Na7 84.15(5) 2 2_554
Na1 Na3 Na7 59.21(7) . 2_554
As2 Na3 Na7 59.40(6) . 2_564
As3 Na3 Na7 88.55(4) 2_565 2_564
As3 Na3 Na7 161.49(11) 2 2_564
As5 Na3 Na7 109.89(9) 2 2_564
As5 Na3 Na7 51.46(5) 2_565 2_564
Ga3 Na3 Na7 84.15(5) 2_565 2_564
Ga3 Na3 Na7 149.46(11) 2 2_564
Na1 Na3 Na7 59.21(7) . 2_564
Na7 Na3 Na7 82.24(9) 2_554 2_564
As2 Na3 Na5 53.62(6) . 2_565
As3 Na3 Na5 48.49(5) 2_565 2_565
As3 Na3 Na5 104.84(9) 2 2_565
As5 Na3 Na5 164.43(9) 2 2_565
As5 Na3 Na5 93.10(4) 2_565 2_565
Ga3 Na3 Na5 85.17(5) 2_565 2_565
Ga3 Na3 Na5 145.58(10) 2 2_565
Na1 Na3 Na5 124.02(8) . 2_565
Na7 Na3 Na5 113.02(9) 2_554 2_565
Na7 Na3 Na5 64.83(7) 2_564 2_565
As2 Na3 Na5 53.62(6) . 2
As3 Na3 Na5 104.84(9) 2_565 2
As3 Na3 Na5 48.49(5) 2 2
As5 Na3 Na5 93.10(4) 2 2
As5 Na3 Na5 164.43(9) 2_565 2
Ga3 Na3 Na5 145.58(10) 2_565 2
Ga3 Na3 Na5 85.17(5) 2 2
Na1 Na3 Na5 124.02(8) . 2
Na7 Na3 Na5 64.83(7) 2_554 2
Na7 Na3 Na5 113.02(9) 2_564 2
Na5 Na3 Na5 76.74(8) 2_565 2
Ga2 Na4 Ga2 91.76(8) 2_565 2
Ga2 Na4 Ga3 139.97(9) 2_565 2
Ga2 Na4 Ga3 74.82(3) 2 2
Ga2 Na4 Ga3 74.82(3) 2_565 2_565
Ga2 Na4 Ga3 139.97(9) 2 2_565
Ga3 Na4 Ga3 91.40(8) 2 2_565
Ga2 Na4 Ga1 72.87(4) 2_565 2_565
Ga2 Na4 Ga1 136.68(10) 2 2_565
Ga3 Na4 Ga1 140.64(10) 2 2_565
Ga3 Na4 Ga1 75.77(4) 2_565 2_565
Ga2 Na4 Ga1 136.68(10) 2_565 2
Ga2 Na4 Ga1 72.87(4) 2 2
Ga3 Na4 Ga1 75.77(4) 2 2
Ga3 Na4 Ga1 140.64(10) 2_565 2
Ga1 Na4 Ga1 90.78(7) 2_565 2
Ga2 Na4 As3 177.87(10) 2_565 2
Ga2 Na4 As3 88.89(2) 2 2
Ga3 Na4 As3 42.16(3) 2 2
Ga3 Na4 As3 105.92(9) 2_565 2
Ga1 Na4 As3 105.31(8) 2_565 2
Ga1 Na4 As3 41.73(3) 2 2
Ga2 Na4 As3 88.89(2) 2_565 2_565
Ga2 Na4 As3 177.87(10) 2 2_565
Ga3 Na4 As3 105.92(9) 2 2_565
Ga3 Na4 As3 42.16(3) 2_565 2_565
Ga1 Na4 As3 41.73(3) 2_565 2_565
Ga1 Na4 As3 105.31(8) 2 2_565
As3 Na4 As3 90.40(8) 2 2_565
Ga2 Na4 As6 104.89(8) 2_565 2
Ga2 Na4 As6 41.46(3) 2 2
Ga3 Na4 As6 41.96(3) 2 2
Ga3 Na4 As6 105.05(8) 2_565 2
Ga1 Na4 As6 177.40(10) 2_565 2
Ga1 Na4 As6 90.05(2) 2 2
As3 Na4 As6 76.91(4) 2 2
As3 Na4 As6 140.20(10) 2_565 2
Ga2 Na4 As6 41.46(3) 2_565 2_565
Ga2 Na4 As6 104.89(8) 2 2_565
Ga3 Na4 As6 105.05(8) 2 2_565
Ga3 Na4 As6 41.96(3) 2_565 2_565
Ga1 Na4 As6 90.05(2) 2_565 2_565
Ga1 Na4 As6 177.40(10) 2 2_565
As3 Na4 As6 140.20(10) 2 2_565
As3 Na4 As6 76.91(4) 2_565 2_565
As6 Na4 As6 89.01(7) 2 2_565
Ga2 Na4 As2 40.71(3) 2_565 2_565
Ga2 Na4 As2 102.96(8) 2 2_565
Ga3 Na4 As2 177.44(7) 2 2_565
Ga3 Na4 As2 91.13(2) 2_565 2_565
Ga1 Na4 As2 40.66(3) 2_565 2_565
Ga1 Na4 As2 102.45(8) 2 2_565
As3 Na4 As2 137.16(9) 2 2_565
As3 Na4 As2 76.25(4) 2_565 2_565
As6 Na4 As2 136.74(10) 2 2_565
As6 Na4 As2 76.65(4) 2_565 2_565
Ga2 Na4 As2 102.96(8) 2_565 2
Ga2 Na4 As2 40.71(3) 2 2
Ga3 Na4 As2 91.13(2) 2 2
Ga3 Na4 As2 177.44(7) 2_565 2
Ga1 Na4 As2 102.45(8) 2_565 2
Ga1 Na4 As2 40.66(3) 2 2
As3 Na4 As2 76.25(4) 2 2
As3 Na4 As2 137.16(9) 2_565 2
As6 Na4 As2 76.65(4) 2 2
As6 Na4 As2 136.74(10) 2_565 2
As2 Na4 As2 86.34(7) 2_565 2
As3 Na5 As2 104.27(7) . 2_554
As3 Na5 As2 104.27(7) . 2_564
As2 Na5 As2 97.29(8) 2_554 2_564
As3 Na5 Ga2 133.37(4) . 2_554
As2 Na5 Ga2 43.06(3) 2_554 2_554
As2 Na5 Ga2 111.10(9) 2_564 2_554
As3 Na5 Ga2 133.37(4) . 2_564
As2 Na5 Ga2 111.10(9) 2_554 2_564
As2 Na5 Ga2 43.06(3) 2_564 2_564
Ga2 Na5 Ga2 93.18(8) 2_554 2_564
As3 Na5 As4 110.76(7) . 2_554
As2 Na5 As4 75.03(3) 2_554 2_554
As2 Na5 As4 144.97(10) 2_564 2_554
Ga2 Na5 As4 41.50(3) 2_554 2_554
Ga2 Na5 As4 107.07(8) 2_564 2_554
As3 Na5 As4 110.76(7) . 2_564
As2 Na5 As4 144.97(10) 2_554 2_564
As2 Na5 As4 75.03(3) 2_564 2_564
Ga2 Na5 As4 107.07(8) 2_554 2_564
Ga2 Na5 As4 41.50(3) 2_564 2_564
As4 Na5 As4 91.69(8) 2_554 2_564
As3 Na5 Na2 95.43(9) . .
As2 Na5 Na2 125.94(6) 2_554 .
As2 Na5 Na2 125.94(6) 2_564 .
Ga2 Na5 Na2 87.77(7) 2_554 .
Ga2 Na5 Na2 87.77(7) 2_564 .
As4 Na5 Na2 50.91(5) 2_554 .
As4 Na5 Na2 50.91(5) 2_564 .
As3 Na5 Na6 60.63(6) . 2_564
As2 Na5 Na6 164.81(10) 2_554 2_564
As2 Na5 Na6 88.73(4) 2_564 2_564
Ga2 Na5 Na6 146.05(10) 2_554 2_564
Ga2 Na5 Na6 82.76(5) 2_564 2_564
As4 Na5 Na6 107.62(9) 2_554 2_564
As4 Na5 Na6 50.14(5) 2_564 2_564
Na2 Na5 Na6 58.48(6) . 2_564
As3 Na5 Na6 60.63(6) . 2_554
As2 Na5 Na6 88.73(4) 2_554 2_554
As2 Na5 Na6 164.81(10) 2_564 2_554
Ga2 Na5 Na6 82.76(5) 2_554 2_554
Ga2 Na5 Na6 146.05(10) 2_564 2_554
As4 Na5 Na6 50.14(5) 2_554 2_554
As4 Na5 Na6 107.62(9) 2_564 2_554
Na2 Na5 Na6 58.48(6) . 2_554
Na6 Na5 Na6 82.24(9) 2_564 2_554
As3 Na5 Na8 151.62(11) . 6_556
As2 Na5 Na8 94.28(7) 2_554 6_556
As2 Na5 Na8 94.28(7) 2_564 6_556
Ga2 Na5 Na8 53.72(5) 2_554 6_556
Ga2 Na5 Na8 53.72(5) 2_564 6_556
As4 Na5 Na8 53.35(5) 2_554 6_556
As4 Na5 Na8 53.35(5) 2_564 6_556
Na2 Na5 Na8 56.19(8) . 6_556
Na6 Na5 Na8 99.19(8) 2_564 6_556
Na6 Na5 Na8 99.19(8) 2_554 6_556
As3 Na5 Na3 54.73(6) . 2_564
As2 Na5 Na3 106.45(8) 2_554 2_564
As2 Na5 Na3 49.56(5) 2_564 2_564
Ga2 Na5 Na3 146.47(10) 2_554 2_564
Ga2 Na5 Na3 86.09(5) 2_564 2_564
As4 Na5 Na3 165.47(9) 2_554 2_564
As4 Na5 Na3 94.43(4) 2_564 2_564
Na2 Na5 Na3 125.63(7) . 2_564
Na6 Na5 Na3 67.16(7) 2_564 2_564
Na6 Na5 Na3 115.35(9) 2_554 2_564
Na8 Na5 Na3 139.48(5) 6_556 2_564
As4 Na6 As1 105.41(7) . 2_565
As4 Na6 As1 105.41(7) . 2
As1 Na6 As1 96.45(8) 2_565 2
As4 Na6 Ga1 132.33(4) . 2_565
As1 Na6 Ga1 42.44(3) 2_565 2_565
As1 Na6 Ga1 111.38(9) 2 2_565
As4 Na6 Ga1 132.33(4) . 2
As1 Na6 Ga1 111.38(9) 2_565 2
As1 Na6 Ga1 42.44(3) 2 2
Ga1 Na6 Ga1 95.32(8) 2_565 2
As4 Na6 As3 109.39(7) . 2
As1 Na6 As3 145.13(9) 2_565 2
As1 Na6 As3 76.44(3) 2 2
Ga1 Na6 As3 107.89(8) 2_565 2
Ga1 Na6 As3 42.41(3) 2 2
As4 Na6 As3 109.39(7) . 2_565
As1 Na6 As3 76.44(3) 2_565 2_565
As1 Na6 As3 145.13(9) 2 2_565
Ga1 Na6 As3 42.41(3) 2_565 2_565
Ga1 Na6 As3 107.89(8) 2 2_565
As3 Na6 As3 90.02(7) 2 2_565
As4 Na6 Na2 53.67(6) . 2_565
As1 Na6 Na2 52.17(5) 2_565 2_565
As1 Na6 Na2 113.77(9) 2 2_565
Ga1 Na6 Na2 83.67(4) 2_565 2_565
Ga1 Na6 Na2 153.78(11) 2 2_565
As3 Na6 Na2 161.24(11) 2 2_565
As3 Na6 Na2 89.03(4) 2_565 2_565
As4 Na6 Na2 53.67(6) . 2
As1 Na6 Na2 113.77(9) 2_565 2
As1 Na6 Na2 52.17(5) 2 2
Ga1 Na6 Na2 153.78(11) 2_565 2
Ga1 Na6 Na2 83.67(4) 2 2
As3 Na6 Na2 89.03(4) 2 2
As3 Na6 Na2 161.24(11) 2_565 2
Na2 Na6 Na2 85.90(9) 2_565 2
As4 Na6 Na5 59.61(6) . 2
As1 Na6 Na5 165.00(10) 2_565 2
As1 Na6 Na5 89.14(4) 2 2
Ga1 Na6 Na5 146.49(10) 2_565 2
Ga1 Na6 Na5 82.05(5) 2 2
As3 Na6 Na5 49.79(5) 2 2
As3 Na6 Na5 106.53(9) 2_565 2
Na2 Na6 Na5 112.85(10) 2_565 2
Na2 Na6 Na5 59.49(7) 2 2
As4 Na6 Na5 59.61(6) . 2_565
As1 Na6 Na5 89.14(4) 2_565 2_565
As1 Na6 Na5 165.00(10) 2 2_565
Ga1 Na6 Na5 82.05(5) 2_565 2_565
Ga1 Na6 Na5 146.49(10) 2 2_565
As3 Na6 Na5 106.53(9) 2 2_565
As3 Na6 Na5 49.79(5) 2_565 2_565
Na2 Na6 Na5 59.49(7) 2_565 2_565
Na2 Na6 Na5 112.85(10) 2 2_565
Na5 Na6 Na5 82.23(9) 2 2_565
As4 Na6 Na7 144.34(11) . .
As1 Na6 Na7 55.11(5) 2_565 .
As1 Na6 Na7 55.11(5) 2 .
Ga1 Na6 Na7 56.32(5) 2_565 .
Ga1 Na6 Na7 56.32(5) 2 .
As3 Na6 Na7 95.40(7) 2 .
As3 Na6 Na7 95.40(7) 2_565 .
Na2 Na6 Na7 103.34(8) 2_565 .
Na2 Na6 Na7 103.34(8) 2 .
Na5 Na6 Na7 137.43(5) 2 .
Na5 Na6 Na7 137.43(5) 2_565 .
As5 Na7 As1 106.55(7) 1_556 2
As5 Na7 As1 106.55(7) 1_556 2_565
As1 Na7 As1 96.51(8) 2 2_565
As5 Na7 Ga1 133.17(4) 1_556 2
As1 Na7 Ga1 42.13(3) 2 2
As1 Na7 Ga1 110.28(9) 2_565 2
As5 Na7 Ga1 133.17(4) 1_556 2_565
As1 Na7 Ga1 110.28(9) 2 2_565
As1 Na7 Ga1 42.13(3) 2_565 2_565
Ga1 Na7 Ga1 93.65(8) 2 2_565
As5 Na7 As2 108.81(7) 1_556 2
As1 Na7 As2 75.29(3) 2 2
As1 Na7 As2 144.59(10) 2_565 2
Ga1 Na7 As2 42.24(3) 2 2
Ga1 Na7 As2 107.73(8) 2_565 2
As5 Na7 As2 108.81(7) 1_556 2_565
As1 Na7 As2 144.59(10) 2 2_565
As1 Na7 As2 75.29(3) 2_565 2_565
Ga1 Na7 As2 107.73(8) 2 2_565
Ga1 Na7 As2 42.24(3) 2_565 2_565
As2 Na7 As2 91.52(8) 2 2_565
As5 Na7 Na1 53.83(6) 1_556 2_565
As1 Na7 Na1 114.51(10) 2 2_565
As1 Na7 Na1 53.06(5) 2_565 2_565
Ga1 Na7 Na1 153.94(11) 2 2_565
Ga1 Na7 Na1 84.58(4) 2_565 2_565
As2 Na7 Na1 161.16(11) 2 2_565
As2 Na7 Na1 88.35(4) 2_565 2_565
As5 Na7 Na1 53.83(6) 1_556 2
As1 Na7 Na1 53.06(5) 2 2
As1 Na7 Na1 114.51(10) 2_565 2
Ga1 Na7 Na1 84.58(4) 2 2
Ga1 Na7 Na1 153.94(11) 2_565 2
As2 Na7 Na1 88.35(4) 2 2
As2 Na7 Na1 161.16(11) 2_565 2
Na1 Na7 Na1 85.80(9) 2_565 2
As5 Na7 Na3 57.90(6) 1_556 2_565
As1 Na7 Na3 164.44(10) 2 2_565
As1 Na7 Na3 88.97(4) 2_565 2_565
Ga1 Na7 Na3 147.73(10) 2 2_565
Ga1 Na7 Na3 83.48(5) 2_565 2_565
As2 Na7 Na3 108.18(9) 2 2_565
As2 Na7 Na3 50.94(5) 2_565 2_565
Na1 Na7 Na3 58.02(7) 2_565 2_565
Na1 Na7 Na3 111.45(10) 2 2_565
As5 Na7 Na3 57.90(6) 1_556 2
As1 Na7 Na3 88.97(4) 2 2
As1 Na7 Na3 164.44(10) 2_565 2
Ga1 Na7 Na3 83.48(5) 2 2
Ga1 Na7 Na3 147.73(10) 2_565 2
As2 Na7 Na3 50.94(5) 2 2
As2 Na7 Na3 108.18(9) 2_565 2
Na1 Na7 Na3 111.45(10) 2_565 2
Na1 Na7 Na3 58.02(7) 2 2
Na3 Na7 Na3 82.24(9) 2_565 2
As5 Na7 Na6 146.18(11) 1_556 .
As1 Na7 Na6 55.14(5) 2 .
As1 Na7 Na6 55.14(5) 2_565 .
Ga1 Na7 Na6 55.18(5) 2 .
Ga1 Na7 Na6 55.18(5) 2_565 .
As2 Na7 Na6 94.39(7) 2 .
As2 Na7 Na6 94.39(7) 2_565 .
Na1 Na7 Na6 104.41(8) 2_565 .
Na1 Na7 Na6 104.41(8) 2 .
Na3 Na7 Na6 137.62(5) 2_565 .
Na3 Na7 Na6 137.62(5) 2 .
As4 Na8 As4 110.14(7) . 5_656
As4 Na8 As4 110.14(7) . 5_666
As4 Na8 As4 95.36(8) 5_656 5_666
As4 Na8 Ga2 132.18(4) . 5_666
As4 Na8 Ga2 110.74(8) 5_656 5_666
As4 Na8 Ga2 42.52(3) 5_666 5_666
As4 Na8 Ga2 132.18(4) . 5_656
As4 Na8 Ga2 42.52(3) 5_656 5_656
As4 Na8 Ga2 110.74(8) 5_666 5_656
Ga2 Na8 Ga2 95.10(8) 5_666 5_656
As4 Na8 As6 103.83(7) . 5_666
As4 Na8 As6 145.78(9) 5_656 5_666
As4 Na8 As6 76.33(3) 5_666 5_666
Ga2 Na8 As6 42.62(3) 5_666 5_666
Ga2 Na8 As6 108.98(8) 5_656 5_666
As4 Na8 As6 103.83(7) . 5_656
As4 Na8 As6 76.33(3) 5_656 5_656
As4 Na8 As6 145.78(9) 5_666 5_656
Ga2 Na8 As6 108.98(8) 5_666 5_656
Ga2 Na8 As6 42.62(3) 5_656 5_656
As6 Na8 As6 91.95(8) 5_666 5_656
As4 Na8 Na2 96.01(9) . 6_656
As4 Na8 Na2 52.30(5) 5_656 6_656
As4 Na8 Na2 52.30(5) 5_666 6_656
Ga2 Na8 Na2 89.88(7) 5_666 6_656
Ga2 Na8 Na2 89.88(7) 5_656 6_656
As6 Na8 Na2 128.60(5) 5_666 6_656
As6 Na8 Na2 128.60(5) 5_656 6_656
As4 Na8 Na8 58.66(7) . 5_656
As4 Na8 Na8 51.48(5) 5_656 5_656
As4 Na8 Na8 111.83(13) 5_666 5_656
Ga2 Na8 Na8 151.84(14) 5_666 5_656
Ga2 Na8 Na8 83.63(4) 5_656 5_656
As6 Na8 Na8 162.07(13) 5_666 5_656
As6 Na8 Na8 89.09(4) 5_656 5_656
Na2 Na8 Na8 62.03(9) 6_656 5_656
As4 Na8 Na8 58.66(7) . 5_666
As4 Na8 Na8 111.83(13) 5_656 5_666
As4 Na8 Na8 51.48(5) 5_666 5_666
Ga2 Na8 Na8 83.63(4) 5_666 5_666
Ga2 Na8 Na8 151.84(14) 5_656 5_666
As6 Na8 Na8 89.09(4) 5_666 5_666
As6 Na8 Na8 162.07(13) 5_656 5_666
Na2 Na8 Na8 62.03(9) 6_656 5_666
Na8 Na8 Na8 84.54(13) 5_656 5_666
As4 Na8 Na2 52.33(6) . 2
As4 Na8 Na2 88.55(4) 5_656 2
As4 Na8 Na2 162.03(10) 5_666 2
Ga2 Na8 Na2 150.18(11) 5_666 2
Ga2 Na8 Na2 83.86(5) 5_656 2
As6 Na8 Na2 109.63(9) 5_666 2
As6 Na8 Na2 52.15(5) 5_656 2
Na2 Na8 Na2 119.88(7) 6_656 2
Na8 Na8 Na2 57.85(7) 5_656 2
Na8 Na8 Na2 110.86(12) 5_666 2
As4 Na8 Na2 52.33(6) . 2_565
As4 Na8 Na2 162.03(10) 5_656 2_565
As4 Na8 Na2 88.55(4) 5_666 2_565
Ga2 Na8 Na2 83.86(5) 5_666 2_565
Ga2 Na8 Na2 150.18(11) 5_656 2_565
As6 Na8 Na2 52.15(5) 5_666 2_565
As6 Na8 Na2 109.63(9) 5_656 2_565
Na2 Na8 Na2 119.88(7) 6_656 2_565
Na8 Na8 Na2 110.86(12) 5_656 2_565
Na8 Na8 Na2 57.85(7) 5_666 2_565
Na2 Na8 Na2 82.65(9) 2 2_565
As1 Ga1 As2 115.89(4) . .
As1 Ga1 As3 119.19(4) . .
As2 Ga1 As3 124.92(4) . .
As1 Ga1 Na6 68.12(5) . 2_554
As2 Ga1 Na6 131.87(4) . 2_554
As3 Ga1 Na6 72.06(5) . 2_554
As1 Ga1 Na6 68.12(5) . 2_564
As2 Ga1 Na6 131.87(4) . 2_564
As3 Ga1 Na6 72.06(5) . 2_564
Na6 Ga1 Na6 95.32(8) 2_554 2_564
As1 Ga1 Na7 67.24(5) . 2_564
As2 Ga1 Na7 70.20(5) . 2_564
As3 Ga1 Na7 132.95(4) . 2_564
Na6 Ga1 Na7 135.36(7) 2_554 2_564
Na6 Ga1 Na7 68.49(6) 2_564 2_564
As1 Ga1 Na7 67.24(5) . 2_554
As2 Ga1 Na7 70.20(5) . 2_554
As3 Ga1 Na7 132.95(4) . 2_554
Na6 Ga1 Na7 68.49(6) 2_554 2_554
Na6 Ga1 Na7 135.36(7) 2_564 2_554
Na7 Ga1 Na7 93.65(8) 2_564 2_554
As1 Ga1 Na4 134.60(4) . 2_564
As2 Ga1 Na4 72.74(5) . 2_564
As3 Ga1 Na4 69.38(5) . 2_564
Na6 Ga1 Na4 141.41(8) 2_554 2_564
Na6 Ga1 Na4 74.29(6) 2_564 2_564
Na7 Ga1 Na4 76.04(6) 2_564 2_564
Na7 Ga1 Na4 142.85(8) 2_554 2_564
As1 Ga1 Na4 134.60(4) . 2_554
As2 Ga1 Na4 72.74(5) . 2_554
As3 Ga1 Na4 69.38(5) . 2_554
Na6 Ga1 Na4 74.29(6) 2_554 2_554
Na6 Ga1 Na4 141.41(8) 2_564 2_554
Na7 Ga1 Na4 142.85(8) 2_564 2_554
Na7 Ga1 Na4 76.04(6) 2_554 2_554
Na4 Ga1 Na4 90.78(7) 2_564 2_554
As4 Ga2 As2 114.31(4) . .
As4 Ga2 As6 117.77(4) . .
As2 Ga2 As6 127.93(4) . .
As4 Ga2 Na8 68.60(5) . 5_666
As2 Ga2 Na8 131.88(4) . 5_666
As6 Ga2 Na8 70.59(6) . 5_666
As4 Ga2 Na8 68.60(5) . 5_656
As2 Ga2 Na8 131.88(4) . 5_656
As6 Ga2 Na8 70.59(6) . 5_656
Na8 Ga2 Na8 95.11(8) 5_666 5_656
As4 Ga2 Na5 70.19(5) . 2_565
As2 Ga2 Na5 66.09(5) . 2_565
As6 Ga2 Na5 133.38(4) . 2_565
Na8 Ga2 Na5 71.32(6) 5_666 2_565
Na8 Ga2 Na5 138.74(8) 5_656 2_565
As4 Ga2 Na5 70.19(5) . 2
As2 Ga2 Na5 66.09(5) . 2
As6 Ga2 Na5 133.38(4) . 2
Na8 Ga2 Na5 138.74(8) 5_666 2
Na8 Ga2 Na5 71.32(6) 5_656 2
Na5 Ga2 Na5 93.18(8) 2_565 2
As4 Ga2 Na4 134.12(4) . 2_554
As2 Ga2 Na4 73.35(5) . 2_554
As6 Ga2 Na4 71.07(5) . 2_554
Na8 Ga2 Na4 141.60(7) 5_666 2_554
Na8 Ga2 Na4 74.00(6) 5_656 2_554
Na5 Ga2 Na4 139.25(8) 2_565 2_554
Na5 Ga2 Na4 73.41(6) 2 2_554
As4 Ga2 Na4 134.12(4) . 2_564
As2 Ga2 Na4 73.35(5) . 2_564
As6 Ga2 Na4 71.07(5) . 2_564
Na8 Ga2 Na4 74.00(6) 5_666 2_564
Na8 Ga2 Na4 141.60(7) 5_656 2_564
Na5 Ga2 Na4 73.41(6) 2_565 2_564
Na5 Ga2 Na4 139.25(8) 2 2_564
Na4 Ga2 Na4 91.76(8) 2_554 2_564
As5 Ga3 As3 113.79(4) . .
As5 Ga3 As6 124.65(4) . .
As3 Ga3 As6 121.56(4) . .
As5 Ga3 Na3 68.92(6) . 2_554
As3 Ga3 Na3 67.42(6) . 2_554
As6 Ga3 Na3 132.86(4) . 2_554
As5 Ga3 Na3 68.92(6) . 2_564
As3 Ga3 Na3 67.42(6) . 2_564
As6 Ga3 Na3 132.86(4) . 2_564
Na3 Ga3 Na3 94.16(8) 2_554 2_564
As5 Ga3 Na4 133.97(4) . 2_564
As3 Ga3 Na4 69.56(5) . 2_564
As6 Ga3 Na4 70.57(5) . 2_564
Na3 Ga3 Na4 136.90(7) 2_554 2_564
Na3 Ga3 Na4 71.46(6) 2_564 2_564
As5 Ga3 Na4 133.97(4) . 2_554
As3 Ga3 Na4 69.56(5) . 2_554
As6 Ga3 Na4 70.57(5) . 2_554
Na3 Ga3 Na4 71.46(6) 2_554 2_554
Na3 Ga3 Na4 136.90(7) 2_564 2_554
Na4 Ga3 Na4 91.40(8) 2_564 2_554
As5 Ga3 Rb 70.69(2) . 2_564
As3 Ga3 Rb 140.095(13) . 2_564
As6 Ga3 Rb 67.56(2) . 2_564
Na3 Ga3 Rb 138.68(6) 2_554 2_564
Na3 Ga3 Rb 79.17(5) 2_564 2_564
Na4 Ga3 Rb 79.81(5) 2_564 2_564
Na4 Ga3 Rb 137.79(6) 2_554 2_564
As5 Ga3 Rb 70.69(2) . 2_554
As3 Ga3 Rb 140.095(14) . 2_554
As6 Ga3 Rb 67.56(2) . 2_554
Na3 Ga3 Rb 79.17(5) 2_554 2_554
Na3 Ga3 Rb 138.68(6) 2_564 2_554
Na4 Ga3 Rb 137.79(6) 2_564 2_554
Na4 Ga3 Rb 79.81(5) 2_554 2_554
Rb Ga3 Rb 79.75(3) 2_564 2_554
Ga1 As1 Na2 115.94(7) . .
Ga1 As1 Na1 117.09(7) . .
Na2 As1 Na1 126.97(8) . .
Ga1 As1 Na7 70.63(5) . 2_564
Na2 As1 Na7 131.63(4) . 2_564
Na1 As1 Na7 68.71(6) . 2_564
Ga1 As1 Na7 70.63(5) . 2_554
Na2 As1 Na7 131.63(4) . 2_554
Na1 As1 Na7 68.71(6) . 2_554
Na7 As1 Na7 96.51(8) 2_564 2_554
Ga1 As1 Na6 69.44(5) . 2_554
Na2 As1 Na6 69.18(6) . 2_554
Na1 As1 Na6 131.60(4) . 2_554
Na7 As1 Na6 140.07(7) 2_564 2_554
Na7 As1 Na6 69.75(6) 2_554 2_554
Ga1 As1 Na6 69.44(5) . 2_564
Na2 As1 Na6 69.18(6) . 2_564
Na1 As1 Na6 131.60(4) . 2_564
Na7 As1 Na6 69.75(6) 2_564 2_564
Na7 As1 Na6 140.07(7) 2_554 2_564
Na6 As1 Na6 96.45(8) 2_554 2_564
Ga1 As1 Rb 137.565(14) . 5_556
Na2 As1 Rb 71.58(4) . 5_556
Na1 As1 Rb 69.95(4) . 5_556
Na7 As1 Rb 138.06(6) 2_564 5_556
Na7 As1 Rb 74.75(5) 2_554 5_556
Na6 As1 Rb 76.13(5) 2_554 5_556
Na6 As1 Rb 140.05(6) 2_564 5_556
Ga1 As1 Rb 137.565(14) . 5_566
Na2 As1 Rb 71.58(4) . 5_566
Na1 As1 Rb 69.95(4) . 5_566
Na7 As1 Rb 74.75(5) 2_564 5_566
Na7 As1 Rb 138.06(6) 2_554 5_566
Na6 As1 Rb 140.05(6) 2_554 5_566
Na6 As1 Rb 76.13(5) 2_564 5_566
Rb As1 Rb 84.86(3) 5_556 5_566
Ga2 As2 Ga1 113.01(4) . .
Ga2 As2 Na3 130.04(7) . .
Ga1 As2 Na3 116.95(7) . .
Ga2 As2 Na5 70.85(5) . 2_565
Ga1 As2 Na5 131.00(4) . 2_565
Na3 As2 Na5 76.82(6) . 2_565
Ga2 As2 Na5 70.85(5) . 2
Ga1 As2 Na5 131.00(4) . 2
Na3 As2 Na5 76.82(6) . 2
Na5 As2 Na5 97.30(8) 2_565 2
Ga2 As2 Na7 133.37(4) . 2_554
Ga1 As2 Na7 67.56(5) . 2_554
Na3 As2 Na7 69.66(6) . 2_554
Na5 As2 Na7 146.48(7) 2_565 2_554
Na5 As2 Na7 76.00(6) 2 2_554
Ga2 As2 Na7 133.37(4) . 2_564
Ga1 As2 Na7 67.56(5) . 2_564
Na3 As2 Na7 69.66(6) . 2_564
Na5 As2 Na7 76.00(6) 2_565 2_564
Na5 As2 Na7 146.48(7) 2 2_564
Na7 As2 Na7 91.51(8) 2_554 2_564
Ga2 As2 Na4 65.94(5) . 2_554
Ga1 As2 Na4 66.60(5) . 2_554
Na3 As2 Na4 136.49(4) . 2_554
Na5 As2 Na4 136.60(7) 2_565 2_554
Na5 As2 Na4 72.51(6) 2 2_554
Na7 As2 Na4 73.47(6) 2_554 2_554
Na7 As2 Na4 134.08(7) 2_564 2_554
Ga2 As2 Na4 65.94(5) . 2_564
Ga1 As2 Na4 66.60(5) . 2_564
Na3 As2 Na4 136.49(4) . 2_564
Na5 As2 Na4 72.51(6) 2_565 2_564
Na5 As2 Na4 136.60(7) 2 2_564
Na7 As2 Na4 134.08(7) 2_554 2_564
Na7 As2 Na4 73.47(6) 2_564 2_564
Na4 As2 Na4 86.34(7) 2_554 2_564
Ga1 As3 Ga3 117.57(4) . .
Ga1 As3 Na5 114.58(7) . .
Ga3 As3 Na5 127.84(7) . .
Ga1 As3 Na3 132.08(4) . 2_554
Ga3 As3 Na3 68.95(5) . 2_554
Na5 As3 Na3 76.79(7) . 2_554
Ga1 As3 Na3 132.08(4) . 2_564
Ga3 As3 Na3 68.95(5) . 2_564
Na5 As3 Na3 76.79(7) . 2_564
Na3 As3 Na3 95.50(8) 2_554 2_564
Ga1 As3 Na4 68.89(5) . 2_564
Ga3 As3 Na4 68.28(5) . 2_564
Na5 As3 Na4 134.48(4) . 2_564
Na3 As3 Na4 137.15(7) 2_554 2_564
Na3 As3 Na4 71.50(6) 2_564 2_564
Ga1 As3 Na4 68.89(5) . 2_554
Ga3 As3 Na4 68.28(5) . 2_554
Na5 As3 Na4 134.48(4) . 2_554
Na3 As3 Na4 71.50(6) 2_554 2_554
Na3 As3 Na4 137.15(7) 2_564 2_554
Na4 As3 Na4 90.39(8) 2_564 2_554
Ga1 As3 Na6 65.54(5) . 2_554
Ga3 As3 Na6 134.40(4) . 2_554
Na5 As3 Na6 69.59(6) . 2_554
Na3 As3 Na6 77.62(6) 2_554 2_554
Na3 As3 Na6 146.37(7) 2_564 2_554
Na4 As3 Na6 134.40(7) 2_564 2_554
Na4 As3 Na6 72.31(6) 2_554 2_554
Ga1 As3 Na6 65.54(5) . 2_564
Ga3 As3 Na6 134.40(4) . 2_564
Na5 As3 Na6 69.59(6) . 2_564
Na3 As3 Na6 146.37(7) 2_554 2_564
Na3 As3 Na6 77.62(6) 2_564 2_564
Na4 As3 Na6 72.31(6) 2_564 2_564
Na4 As3 Na6 134.40(7) 2_554 2_564
Na6 As3 Na6 90.02(7) 2_554 2_564
Ga2 As4 Na8 116.90(7) . .
Ga2 As4 Na2 126.18(5) . 2_565
Na8 As4 Na2 75.34(7) . 2_565
Ga2 As4 Na2 126.18(5) . 2
Na8 As4 Na2 75.34(7) . 2
Na2 As4 Na2 107.61(9) 2_565 2
Ga2 As4 Na6 118.93(7) . .
Na8 As4 Na6 124.17(8) . .
Na2 As4 Na6 72.58(6) 2_565 .
Na2 As4 Na6 72.58(6) 2 .
Ga2 As4 Na8 68.89(5) . 5_656
Na8 As4 Na8 69.86(7) . 5_656
Na2 As4 Na8 144.91(8) 2_565 5_656
Na2 As4 Na8 67.97(7) 2 5_656
Na6 As4 Na8 132.23(4) . 5_656
Ga2 As4 Na8 68.89(5) . 5_666
Na8 As4 Na8 69.86(7) . 5_666
Na2 As4 Na8 67.97(7) 2_565 5_666
Na2 As4 Na8 144.91(8) 2 5_666
Na6 As4 Na8 132.23(4) . 5_666
Na8 As4 Na8 95.36(8) 5_656 5_666
Ga2 As4 Na5 68.31(5) . 2
Na8 As4 Na5 133.93(4) . 2
Na2 As4 Na5 141.99(8) 2_565 2
Na2 As4 Na5 68.28(7) 2 2
Na6 As4 Na5 70.25(6) . 2
Na8 As4 Na5 70.87(6) 5_656 2
Na8 As4 Na5 137.16(7) 5_666 2
Ga2 As4 Na5 68.31(5) . 2_565
Na8 As4 Na5 133.93(4) . 2_565
Na2 As4 Na5 68.28(7) 2_565 2_565
Na2 As4 Na5 141.99(8) 2 2_565
Na6 As4 Na5 70.25(6) . 2_565
Na8 As4 Na5 137.16(7) 5_656 2_565
Na8 As4 Na5 70.87(6) 5_666 2_565
Na5 As4 Na5 91.69(8) 2 2_565
Ga3 As5 Na1 126.79(5) . 2_554
Ga3 As5 Na1 126.79(5) . 2_564
Na1 As5 Na1 106.32(9) 2_554 2_564
Ga3 As5 Na7 119.00(6) . 1_554
Na1 As5 Na7 71.64(6) 2_554 1_554
Na1 As5 Na7 71.64(6) 2_564 1_554
Ga3 As5 Na1 125.73(6) . 6_656
Na1 As5 Na1 70.92(6) 2_554 6_656
Na1 As5 Na1 70.92(6) 2_564 6_656
Na7 As5 Na1 115.27(8) 1_554 6_656
Ga3 As5 Na3 68.94(5) . 2_554
Na1 As5 Na3 67.22(7) 2_554 2_554
Na1 As5 Na3 141.73(7) 2_564 2_554
Na7 As5 Na3 70.64(6) 1_554 2_554
Na1 As5 Na3 132.79(4) 6_656 2_554
Ga3 As5 Na3 68.94(5) . 2_564
Na1 As5 Na3 141.73(7) 2_554 2_564
Na1 As5 Na3 67.22(7) 2_564 2_564
Na7 As5 Na3 70.64(6) 1_554 2_564
Na1 As5 Na3 132.79(4) 6_656 2_564
Na3 As5 Na3 94.17(9) 2_554 2_564
Ga3 As5 Rb 72.43(3) . 2_564
Na1 As5 Rb 135.96(6) 2_554 2_564
Na1 As5 Rb 71.47(5) 2_564 2_564
Na7 As5 Rb 139.310(16) 1_554 2_564
Na1 As5 Rb 66.94(4) 6_656 2_564
Na3 As5 Rb 140.39(6) 2_554 2_564
Na3 As5 Rb 79.73(5) 2_564 2_564
Ga3 As5 Rb 72.43(3) . 2_554
Na1 As5 Rb 71.47(5) 2_554 2_554
Na1 As5 Rb 135.96(6) 2_564 2_554
Na7 As5 Rb 139.310(15) 1_554 2_554
Na1 As5 Rb 66.94(4) 6_656 2_554
Na3 As5 Rb 79.73(5) 2_554 2_554
Na3 As5 Rb 140.39(6) 2_564 2_554
Rb As5 Rb 80.73(3) 2_564 2_554
Ga2 As6 Ga3 115.01(4) . .
Ga2 As6 Na2 114.25(6) . 6_656
Ga3 As6 Na2 130.74(6) . 6_656
Ga2 As6 Na8 66.79(5) . 5_666
Ga3 As6 Na8 133.26(4) . 5_666
Na2 As6 Na8 68.90(6) 6_656 5_666
Ga2 As6 Na8 66.79(5) . 5_656
Ga3 As6 Na8 133.26(4) . 5_656
Na2 As6 Na8 68.90(6) 6_656 5_656
Na8 As6 Na8 91.95(8) 5_666 5_656
Ga2 As6 Na4 67.47(5) . 2_554
Ga3 As6 Na4 67.47(5) . 2_554
Na2 As6 Na4 134.89(4) 6_656 2_554
Na8 As6 Na4 134.22(7) 5_666 2_554
Na8 As6 Na4 71.90(6) 5_656 2_554
Ga2 As6 Na4 67.47(5) . 2_564
Ga3 As6 Na4 67.47(5) . 2_564
Na2 As6 Na4 134.89(4) 6_656 2_564
Na8 As6 Na4 71.90(6) 5_666 2_564
Na8 As6 Na4 134.22(7) 5_656 2_564
Na4 As6 Na4 89.02(7) 2_554 2_564
Ga2 As6 Rb 138.106(14) . 2_554
Ga3 As6 Rb 73.91(3) . 2_554
Na2 As6 Rb 69.91(4) 6_656 2_554
Na8 As6 Rb 138.49(5) 5_666 2_554
Na8 As6 Rb 77.90(5) 5_656 2_554
Na4 As6 Rb 80.96(5) 2_554 2_554
Na4 As6 Rb 141.02(6) 2_564 2_554
Ga2 As6 Rb 138.106(14) . 2_564
Ga3 As6 Rb 73.91(3) . 2_564
Na2 As6 Rb 69.91(4) 6_656 2_564
Na8 As6 Rb 77.90(5) 5_666 2_564
Na8 As6 Rb 138.49(5) 5_656 2_564
Na4 As6 Rb 141.02(6) 2_554 2_564
Na4 As6 Rb 80.96(5) 2_564 2_564
Rb As6 Rb 83.59(3) 2_554 2_564
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Rb As1 3.5491(9) 5_556
Rb As1 3.5491(9) 5_566
Rb As6 3.5929(9) 2_565
Rb As6 3.5929(9) 2
Rb As5 3.6975(9) 2
Rb As5 3.6975(9) 2_565
Rb Ga3 3.7351(10) 2_565
Rb Ga3 3.7351(10) 2
Rb Na1 3.789(2) 5_556
Rb Na1 3.789(2) 5_566
Rb Na2 3.841(2) 5_566
Rb Na2 3.841(2) 5_556
Na1 As5 2.9921(18) 2_565
Na1 As5 2.9921(18) 2
Na1 As1 3.018(3) .
Na1 As5 3.117(3) 6_556
Na1 Na3 3.474(4) .
Na1 Na7 3.518(3) 2_564
Na1 Na7 3.518(3) 2_554
Na1 Na1 3.546(4) 5_556
Na1 Na1 3.546(4) 5_566
Na1 Rb 3.789(2) 5_556
Na1 Rb 3.789(2) 5_566
Na2 As4 2.9673(18) 2_554
Na2 As4 2.9673(18) 2_564
Na2 As1 2.970(3) .
Na2 As6 3.069(3) 6_556
Na2 Na8 3.476(4) 6_556
Na2 Na6 3.514(3) 2_564
Na2 Na6 3.514(3) 2_554
Na2 Na5 3.552(4) .
Na2 Na8 3.627(3) 2_554
Na2 Na8 3.627(3) 2_564
Na2 Rb 3.841(2) 5_566
Na2 Rb 3.841(2) 5_556
Na3 As2 3.015(3) .
Na3 As3 3.235(2) 2_565
Na3 As3 3.235(2) 2
Na3 As5 3.270(2) 2
Na3 As5 3.270(2) 2_565
Na3 Ga3 3.270(2) 2_565
Na3 Ga3 3.270(2) 2
Na3 Na7 3.641(3) 2_554
Na3 Na7 3.641(3) 2_564
Na3 Na5 3.858(3) 2_565
Na3 Na5 3.858(3) 2
Na4 Ga2 3.336(2) 2_565
Na4 Ga2 3.336(2) 2
Na4 Ga3 3.346(2) 2
Na4 Ga3 3.346(2) 2_565
Na4 Ga1 3.364(2) 2_565
Na4 Ga1 3.364(2) 2
Na4 As3 3.375(2) 2
Na4 As3 3.375(2) 2_565
Na4 As6 3.416(2) 2
Na4 As6 3.416(2) 2_565
Na4 As2 3.500(2) 2_565
Na4 As2 3.500(2) 2
Na5 As3 2.967(3) .
Na5 As2 3.190(2) 2_554
Na5 As2 3.190(2) 2_564
Na5 Ga2 3.296(2) 2_554
Na5 Ga2 3.296(2) 2_564
Na5 As4 3.338(2) 2_554
Na5 As4 3.338(2) 2_564
Na5 Na6 3.641(3) 2_564
Na5 Na6 3.641(3) 2_554
Na5 Na8 3.814(4) 6_556
Na5 Na3 3.858(3) 2_564
Na6 As4 2.970(3) .
Na6 As1 3.211(2) 2_565
Na6 As1 3.211(2) 2
Na6 Ga1 3.240(2) 2_565
Na6 Ga1 3.240(2) 2
Na6 As3 3.386(2) 2
Na6 As3 3.386(2) 2_565
Na6 Na2 3.514(3) 2_565
Na6 Na2 3.514(3) 2
Na6 Na5 3.641(3) 2
Na6 Na5 3.641(3) 2_565
Na6 Na7 3.671(4) .
Na7 As5 3.019(3) 1_556
Na7 As1 3.209(2) 2
Na7 As1 3.209(2) 2_565
Na7 Ga1 3.284(2) 2
Na7 Ga1 3.284(2) 2_565
Na7 As2 3.343(2) 2
Na7 As2 3.343(2) 2_565
Na7 Na1 3.518(3) 2_565
Na7 Na1 3.518(3) 2
Na7 Na3 3.641(3) 2_565
Na7 Na3 3.641(3) 2
Na8 As4 2.967(3) .
Na8 As4 3.239(2) 5_656
Na8 As4 3.239(2) 5_666
Na8 Ga2 3.245(2) 5_666
Na8 Ga2 3.245(2) 5_656
Na8 As6 3.330(2) 5_666
Na8 As6 3.330(2) 5_656
Na8 Na2 3.476(4) 6_656
Na8 Na8 3.560(4) 5_656
Na8 Na8 3.560(4) 5_666
Na8 Na2 3.626(3) 2
Na8 Na2 3.626(3) 2_565
Ga1 As1 2.3347(11) .
Ga1 As2 2.3883(12) .
Ga1 As3 2.4001(12) .
Ga1 Na6 3.240(2) 2_554
Ga1 Na6 3.240(2) 2_564
Ga1 Na7 3.284(2) 2_564
Ga1 Na7 3.284(2) 2_554
Ga1 Na4 3.364(2) 2_564
Ga1 Na4 3.364(2) 2_554
Ga2 As4 2.3508(12) .
Ga2 As2 2.3827(12) .
Ga2 As6 2.3910(12) .
Ga2 Na8 3.245(2) 5_666
Ga2 Na8 3.245(2) 5_656
Ga2 Na5 3.296(2) 2_565
Ga2 Na5 3.296(2) 2
Ga2 Na4 3.336(2) 2_554
Ga2 Na4 3.336(2) 2_564
Ga3 As5 2.3512(12) .
Ga3 As3 2.4175(12) .
Ga3 As6 2.4217(12) .
Ga3 Na3 3.270(2) 2_554
Ga3 Na3 3.270(2) 2_564
Ga3 Na4 3.346(2) 2_564
Ga3 Na4 3.346(2) 2_554
Ga3 Rb 3.7351(10) 2_564
Ga3 Rb 3.7351(10) 2_554
As1 Na7 3.209(2) 2_564
As1 Na7 3.209(2) 2_554
As1 Na6 3.211(2) 2_554
As1 Na6 3.211(2) 2_564
As1 Rb 3.5491(9) 5_556
As1 Rb 3.5491(9) 5_566
As2 Na5 3.190(2) 2_565
As2 Na5 3.190(2) 2
As2 Na7 3.343(2) 2_554
As2 Na7 3.343(2) 2_564
As2 Na4 3.500(2) 2_554
As2 Na4 3.500(2) 2_564
As3 Na3 3.235(2) 2_554
As3 Na3 3.235(2) 2_564
As3 Na4 3.375(2) 2_564
As3 Na4 3.375(2) 2_554
As3 Na6 3.386(2) 2_554
As3 Na6 3.386(2) 2_564
As4 Na2 2.9673(18) 2_565
As4 Na2 2.9673(18) 2
As4 Na8 3.239(2) 5_656
As4 Na8 3.239(2) 5_666
As4 Na5 3.338(2) 2
As4 Na5 3.338(2) 2_565
As5 Na1 2.9921(18) 2_554
As5 Na1 2.9921(18) 2_564
As5 Na7 3.019(3) 1_554
As5 Na1 3.117(3) 6_656
As5 Na3 3.270(2) 2_554
As5 Na3 3.270(2) 2_564
As5 Rb 3.6975(9) 2_564
As5 Rb 3.6975(9) 2_554
As6 Na2 3.069(3) 6_656
As6 Na8 3.330(2) 5_666
As6 Na8 3.330(2) 5_656
As6 Na4 3.416(2) 2_554
As6 Na4 3.416(2) 2_564
As6 Rb 3.5930(9) 2_554
As6 Rb 3.5930(9) 2_564
